1 Bull. Mater. Sci., Vol. 31, No. 7, December 2008, pp Indian Academy of Sciences. Facile hydrothermal route to the controlled synthesis of α-fe 2 O 3 1-D nanostructures LIXIA YANG*, YING LIANG, HOU CHEN, LINGYAN KONG and WEI JIANG School of Chemistry and Materials Science, Ludong University, Yantai , China MS received 15 April 2008 Abstract. Single-crystalline α-fe 2 O 3 1-D nanostructures can be obtained via a facile one-step hydrothermal synthetic route. It was found that the introduction of SnCl 4 played a key role in determining the composition and morphology of α-fe 2 O 3. The addition of SnCl 4 favours the formation of Fe 2 O 3 rather than FeOOH, and the morphology can be tuned from nanorod to double-shuttle as the increase of SnCl 4 concentration. The products were characterized by X-ray powder diffraction (XRD), transmission electron microscopy (TEM) and selectedarea electron diffraction (SAED). This simple method does not need any seed, catalyst, or template, thus is promising for large-scale and low-cost production. Keywords. Fe 2 O 3 ; hydrothermal; morphology; nanostructure. 1. Introduction Iron oxides represent an important type of materials capable of use in a wide range of applications, such as catalysis (Rumyantseva et al 2006), sensors (Kotsikau et al 2004; Chen et al 2005; Wu C Z et al 2006), in magnetic devices (Cao et al 2005; Wu J J et al 2006), and in rechargeable lithium batteries (Wu C Z et al 2006). The properties of Fe 2 O 3 are determined predominantly by crystal structure, composition, particle size and morphology. Therefore, the synthesis of Fe 2 O 3 with well controlled composition, size and shape is of great significance for their applications. Since the discovery of carbon nanotubes in 1991, one-dimensional (1-D) nanostructures have aroused intensified interest because of the unique size- and shapedependent properties for future technological applications. α-fe 2 O 3 is the most stable ion oxide under ambient conditions. It is expected that 1-D nanostructures of Fe 2 O 3 will find new applications or improve the performance of existing applications. There have been many reports on the preparation of α-fe 2 O 3. α-fe 2 O 3 nanowire arrays were grown by a vapour-solid route via the tip-growth mechanism (Chueh et al 2006). Large arrays of aligned α-fe 2 O 3 nanotubes were prepared by a templating technique through thermal decomposition of an analytical Fe(NO 3 ) 3 precursor within an anodic alumina membrane. Tang et al (2006) reported the synthesis of α-fe 2 O 3 nanorods through the calcination of FeOOH nanorods precursor. Ordered mesoporous α-fe 2 O 3 with crystalline walls was prepared through silica template (Jiao et al 2006). Zhu et al (2006) reported the synthesis of novel 3D urchin-like α-fe 2 O 3 superstructures. However, there are a few reports dedicated to the synthesis of α-fe 2 O 3 1-D aggregated nanostructures. Herein, we demonstrate that α-fe 2 O 3 nanorods and double-shuttles consisting of nanoparticles can be synthesized through the introduction of SnCl 4 by one-step hydrothermal method, which avoids the subsequent procedure for the removal of the surfactant or template to synthesize one-dimensional aggregated nanostructures. *Author for correspondence Figure 1. XRD pattern of the obtained product. 919
2 920 Lixia Yang et al Figure 2. (a) TEM image of the product, (b) EDS pattern, (c) a single nanorod of the product and (d) HRTEM image from (c) and the inset of (c) is the corresponding SAED pattern. 2. Experimental Hydrous ferric chloride (FeCl 3 6H 2 O), hydrous tin chloride (SnCl 4 5H 2 O) and sodium hydroxide (NaOH) were of analytical grade and used as received without further purification. In a typical experimental procedure, 0 33 mmol SnCl 4 and 0 33 mmol FeCl 3 were dissolved in 30 ml distilled water at room temperature. 10 ml 2M NaOH solution was added to the above solution and yellow-brown precipitates occurred immediately. Then the mixture solution was transferred into a commercial stainless steel Teflon-lined autoclave of 50 ml capacity. The autoclave was maintained at a temperature of 180 C for 12 h without stirring and shaking during heating and then was allowed to cool to ambient temperature naturally. The products were collected by centrifugation, washed twice with distilled water and absolute ethanol respectively, and finally dried in air at 60 C. The XRD pattern of prepared powder sample was collected using a Rigaku D/Max-2200PC X-ray diffractometer using CuKα radiation (λ = Å) and a graphite monochromator. Transmission electron microscopy (TEM)
3 Facile hydrothermal route to the controlled synthesis of α-fe 2 O 3 1-D nanostructures 921 Figure 3. (a, e) TEM images of the products prepared by the addition of 0 66 mmol SnCl 4, (b) a single double-shuttle of the product, (c) higher magnification of part of (b); (d) HRTEM image from (c); the inset of (b) is the corresponding SAED pattern and (f) is the corresponding SAED pattern of (e).
4 922 Lixia Yang et al and selected-area electron diffraction (SAED) were obtained using a JEOL JEM-2100F field emission transmission electron microscope. 3. Results and discussion Figure 1 shows the typical XRD pattern of the product. All the reflections of the XRD pattern can be indexed to the single phase of α-fe 2 O 3 with hexagonal structure (JCPDS Card No ). No other phases of SnO 2 or FeOOH were found in the XRD pattern. The morphology of the as-prepared sample was investigated by TEM, as shown in figure 2. One can see α- Fe 2 O 3 nanorods with diameters of ~ 100 nm and lengths up to 1 μm. Each nanowire is straight and has relatively sharp tips at the two ends. Energy dispersive spectroscopy (EDS) shows that the nanorods consisted of tin, iron and oxygen (copper came from copper grid of TEM sample holder) (as shown in figure 2b). Selected area electron diffraction (SAED) patterns taken from different positions from an individual nanorod or different α-fe 2 O 3 nanorods were essentially the same, indicating that α- Fe 2 O 3 nanorods were single-crystalline. Figure 2c shows a typical single nanorod and its corresponding SAED pattern (inset of figure 2c). The SAED pattern can be indexed as the [00-1] zone axis of hexagonal α-fe 2 O 3, which is consistent with the XRD result (figure 1). Figure 2d shows the high-resolution TEM (HRTEM) micrograph of an individual nanorod. The visible lattice fringes further confirm that the as-obtained nanorods are single crystals. The addition of SnCl 4 played a key role in the controlled formation of α-fe 2 O 3 nanorods. We carried out the experiment without the use of SnCl 4 with equal amounts of FeCl 3 and NaOH concentrations at 180 C for 12 h. Only FeOOH nanobelts formed, which means that the introduction of SnCl 4 caused the formation of α-fe 2 O 3 instead of FeOOH. We also tried to increase the addition of SnCl 4 concentration to 0 66 mmol, and a single phase of α-fe 2 O 3 was still obtained, with the occurrence of Sn as evidenced by EDS. However, the morphology of α-fe 2 O 3 was double-shuttle as shown in figure 3, and the shuttles have a rough surface with sawtooth structure (figure 3c). It is amazing that SAED pattern taken along the  zone axis reveals that the double-shuttles are singlecrystalline in nature. Shown in figure 3d is the corresponding high-resolution transmission electron microscopy (HRTEM) image and the corresponding SAED pattern. Like the XRD profile, the HRTEM image and the SAED pattern may also be indexed to hexagonal phase of α-fe 2 O 3. The observed lattice spacings of and nm correspond to the (012) and (104) planes of hexagonal α-fe 2 O 3, respectively. It is different from the product prepared by adding 0 33 mmol SnCl 4, which gives single crystal nanorod morphology. From the sawtooth morphology we can speculate that the formation of 1-D nanostructure may have come from the nanoparticle aggregation, at the same time oriented aggregation and particle fusion may have occurred in the process since the SAED pattern shows a single crystal diffraction pattern and no obvious particle boundary was found from HRTEM. In addition, the formation of double-shuttles of α-fe 2 O 3 nanostructures accompanied by the occurrence of some tidy nanoparticles, are as shown in figure 3e. The effect of SnCl 4 addition on the morphology of α- Fe 2 O 3 is obvious, but what is the existence of Sn? it is clear that Sn is present with the formation of α-fe 2 O 3 phase on the basis of EDS, but XRD diffraction peaks give no diffraction peaks of Sn or corresponding oxides. From the corresponding SAED pattern (figure 3f) focused on the areas of large amount of nanoparticles, one can see the intense diffraction rings of polycrystals, which indicates the formation of well-crystallized product. According to the index calculation and the EDS result, we believe that the nanoparticle phase was SnO 2. Due to the low content of SnO 2, the diffraction peaks cannot be found in the XRD pattern. Hence, the final products should be a mixture of α-fe 2 O 3 SnO 2, with α-fe 2 O 3 as the main phase. (1 x)α-fe 2 O 3 xsno 2 composite has been reported by Sorescu et al (2004), but the morphology of α-fe 2 O 3 was different from the present study. It is believed that the addition of SnCl 4 has a key influence on both the composition and morphology of the products, However, detailed formation mechanism of α-fe 2 O 3 nanostructures still needs to be further studied. 4. Conclusions In summary, we have successfully developed a facile hydrothermal synthetic route to single-crystalline Sn-doped α-fe 2 O 3 nanostructure. The introduction of SnCl 4 has a key influence on both the composition and morphology of α-fe 2 O 3. The addition of SnCl 4 favours the formation of Fe 2 O 3 rather than FeOOH, and the morphology can be tuned from nanorod to double-shuttle as the increase of SnCl 4 concentration. This simple method does not need any seed, catalyst, or template, thus is promising for large-scale and low-cost production. The method demonstrated in this paper may also be extended to the fabrication of other doped materials. Acknowledgements The authors are grateful for the financial support by the Natural Science Foundation of Ludong University ((Nos LY , L , , ), the Youth Science Foundation of Shandong Province (Nos 2005BS 11010), the Natural Science Foundation of Shandong Province (Nos Q2006F05, Y2005F11), the Applied Project of Yantai City (No ), and the Applied Pro-
5 Facile hydrothermal route to the controlled synthesis of α-fe 2 O 3 1-D nanostructures 923 ject of Educational Bureau of Shandong province (Nos j05d03, j04b02). References Cao M, Liu T, Gao S, Sun G, Wu X, Hu C and Wang Z L 2005 Angew. Chem. Int. Ed Chen J, Xu L, Li W and Gou X 2005 Adv. Mater Chueh Y L, Lai M W, Liang J Q, Chou L J and Wang Z L 2006 Adv. Funct. Mater Jiao F, Harrison A, Jumas J C, Chadwick A V, Kockelmann W and Bruce P G 2006 J. Am. Chem. Soc Kotsikau D, Ivanovskaya M, Orlik D and Falasconi M 2004 Sensor Actuat. B Rumyantseva M et al 2006 Sensor Actuat. B Sorescu M, Diamandescu L, Tarabasanu-Mihaila D, Teodorescu V S and Howard B H 2004 J. Phys. Chem. Solids Tang B, Wang G, Zhuo L, Ge J and Cui L 2006 Inorg. Chem Wu C Z, Yin P, Zhu X, Yang C O and Xie Y 2006 J. Phys. Chem. B Wu J J, Lee Y L, Chiang H H and Wong D K P 2006 J. Phys. Chem. B Zhu L P, Xiao H M, Liu X M and Fu S Y 2006 J. Mater. Chem